2 Outline Fundamentals of Metal Forming Bulk deformation Sheet metalworking
3 Plastic Deformation Max Load Plastic region A Elastic region Prior to True stress (TS), the stress in the specimen is uniformly distributed.After TS, necking occurs with localization of the deformation to the necking area, which will rapidly go to failure.
4 Temperature in metal forming Hot & Cold WorkingSee MoviesAnswer.Better accuracyBetter Surface finishingStrain hardening increase strengthCosts
5 Preferred Orientation Plastic deformation of idealized (equiaxed) grains in a specimen subjected to compression (such as occurs in the rolling or forging of metals): (a) before deformation; and (b) after deformation. Note hte alignment of grain boundaries along a horizontal direction; this effect is known as preferred orientation.
7 Cold Working Metal forming performed at room temp or slightly above DisadvantageHigher forces are requiredCare the surfaceDuctility is limited.AdvantageBetter accuracyBetter Surface finishingStrain hardening increase strengthCosts
8 Cracks(a)(b)(c)Figure (a) and (b) The effect of elongated inclusions (stringers) on cracking, as a function of the direction of bending with respect to the original rolling direction of the sheet. (c) Cracks on the outer surface of an aluminum strip bent to an angle of 90o. Note the narrowing of the tope surface due to the Poisson effect.
9 Hot working T above Recrystallization Temp. 0. 5Tm < T < 0.75Tm) AdvantageThe shape can be significantly alteredLower forces are requiredFracture can be reducedStrength properties are generally isotropicNo strengthing of the part occurs from work hardeningDisadvantageLower dimensional accuracy, higher energy, poorer surface finishShorter tool life
10 Warm Working Advantage Lower forces are required 0.3Tm < T < 0.5TmAdvantageLower forces are requiredMore intricate work geometries possibleThe need for annealing may be reduced
11 Isothermal Cracking - Raising strength leading to high residual stress For high speed steel, titanium alloy, good hot hardnessQuick heat transfer- Raising strength leading to high residual stressCracking
12 Metal forming process 1. Bulk deformation processes 2. Sheet metal working processes
17 Sheet Metalworking• Deep drawing• Bending• Shearing
18 Forging[Heated] metal is beaten with a heavy hammer to give it the required shapeHot forging,open-die
19 Forging(a)(b)Figure (a) Schematic illustration of the steps involved in forging a bevel gear with a shaft. Source: Forging Industry Association. (b) Landing-gear components for the C5A and C5B transport aircraft, made by forging. Source: Wyman-Gordon Company.
20 Quality of forged parts Surface finish/Dimensional control:Better than casting (typically)Stronger/tougher than cast/machined parts of same material[source:www.scotforge.com]
21 Grain Flow Pattern of Pierced Round Billet Figure A pierced round billet, showing grain flow pattern. Source: Courtesy of Ladish Co., Inc.
22 Grain Flow ComparisonFigure A part made by three different processes, showing grain flow. (a) casting, (b) machining, (c) forging. Source: Forging Industry Association.
23 UpsettingFigure (a) Solid cylindrical billet upset between two flat dies. (b) Uniform deformation of the billet without friction. (c) Deformation with friction. Note barreling of the billet caused by friction forces at the billet-die interfaces.
24 Impression-Die Forging Figure Stages in impression-die forging of a solid round billet. Note the formation of flash, which is excess metal that is subsequently trimmed off (see Fig. 14.8).
25 Forging a Connecting Rod Figure (a) Stages in forging a connecting rod for an internal combustion engine. Note the amount of flash required to ensure proper filling of the die cavities. (b) Fullering, and (c) edging operations to distribute the material when preshaping the blank for forging.
26 Trimming Flash from a Forged Part Figure. Trimming flash from a forged part. Note that the thin material at the center is removed by punching.
30 Comparison of Forging With and Without Flash Figure Comparison of closed-die forging to precision or flashless forging of a cylindrical billet. Source: H. Takemasu, V. Vazquez, B. Painter, and T. Altan.
31 Unit Cost in ForgingFigure Typical unit cost (cost per piece) in forging; note how the setup and the tooling costs per piece decrease as the number of pieces forged increases, if all pieces use the same die.
32 Relative Unit Costs of a Small Connecting Rod Figure .Relative unit costs of a small connecting rod made by various forging and casting processes. Note that, for large quantities, forging is more economical. Sand casting is the more economical process for fewer than about 20,000 pieces.
33 Rolling Important Applications: Steel Plants, Raw stock production (sheets, tubes, Rods, etc.)Screw manufacture
43 Roll-ForgingFigure Two examples of the roll-forging operation, also known as cross-rolling. Tapered leaf springs and knives can be made by this process. Source: (a) J. Holub; (b) reprinted with permission of General Motors Corporation.
44 Roll piercing Compressive Force Rolls Tensile Finished Stresses Tube MandrelTensileFinishedStressesTubeStarting Cylinder
45 Friction and lubrication Friction is undesirable;Metal flow in the work is retardedThe forces to perform are increasedRapid wear of toolingSticking
46 Lubrication Mineral oils Graphite Glass Graphite in water or mineral oil is a common for hot forging
47 Sheet Metal ProcessesRaw material: sheets of metal, rectangular, largeRaw material Processing: Rolling (anisotropic properties)Processes:ShearingPunchingBendingDeep drawing
48 Bending Body of Olympus E-300 camera component with multiple bending operationscomponent with punching,bending, drawing operations[image source: dpreview.com]
49 ShearingA large scissors action, cutting the sheet along a straight lineMain use: to cut large sheet into smaller sizes for making parts.
50 Punching Cutting tool is a round/rectangular punch, that goes through a hole, or die of same shape
51 PunchingMain uses: cutting holes in sheets; cutting sheet to required shapenesting of partstypical punched partExercise: how to determine optimal nesting?
55 C = clearance,a = allowancet = Thickness (plate)C = at
56 How to handle springback: Bending: springback (a) Compensation: the metal is bent by a larger angle(b) Coining the bend:at end of bend cycle, tool exerts large force, dwellscoining: press down hard, wait, release
Your consent to our cookies if you continue to use this website.